# 18th relationships between bond's grindability (g ) and ... ?· 18th international mining congress...

Post on 28-Jun-2018

212 views

Embed Size (px)

TRANSCRIPT

18th International Mining Congress and Exhibition of Turkey-IMCET 2003,

(1984) for the variation of the specific rate of breakage S; with particle size is

(3)

where, X, is the upper limits of the size interval indexed by i, mm, and ax and a are model parameters that depend on the properties of the material and the grinding conditions.

On breakage, particles of given size produce a set of primary daughter fragments, which are mixed into the bulk of the powder and then, in turn, have a probability of being refractured. The set of primary daughter fragments from breakage of size j can be represented by b,.,, where bM is the fraction of size j material, which appears in size /' on primary fracture, n > i >j. It is convenient to represent these values in cumulative form.

(4)

where, B,, is the sum fraction of material less than the upper size of size interval i resulting from primary breakage of size / material: />,-.,= Bu - ,+/., . Austin et al. ( 1981 ) have shown that the values of BM can be estimated from a size analysis of the product from short time grinding of a starling mill charge predominantly in size j (the one-size fraction BI1 method). The equation used is,

(5)

where, P,(t) is the fraction by weight in the mill charge less than size X, at time t. Bu, can be fitted to an empirical function (Austin and Luckie, 1972 ).

(6)

where

(7)

where , cf>, y, and are model parameters that depend on the properties of the material. It is found that, B functions are the same for different ball filling ratios, mill diameters, etc. (Austin et al., 1984). If B,.| values are independent of the initial size, i.e. dimensionally normalizable, then 5 is zero.

3 MATERIALS AND METHOD

3.1 Material

Six limestone samples taken from different regions of Turkey were used as the experimental materials.

The chemical properties of the limestone samples arc presented in Table 1.

Table I. Chemical composition of limestone samples using in experiments.

Oxides (%) C;iO SiO AhO, He :0, MsO SO, NibO K,0 Loss un ignition

Gl

31.03 0.05 0.90 0.00

22.42 0.02 0.07 0.10

45 24

G2

39.09 1.65 1.37 0.00 13.92 0.03 0.07 0.16

43.05

G3

53.56 0.08 1.27 0.00 0.75 0.03 0.06 0.09

43 41

Y

55.43 0.59 0.99 0.00 0.40 0.12 0.05 0.10

42.05

Y2

57.20 0.05 0.90 0.00 0.22 0.02 0.05 0.09

42.74

Y3

48.99 10.60 1.07 0.59 1 I I 0.09 0.04 0.08

38.72

3.2 The test of standard ball mill Bond grindability

The standard Bond grindability test is a closed-cycle dry grinding and screening process, which is carried out until steady state condition is obtained. This test was described as follow (Bond and Maxson, 1943: Yap ct al., 1982; Austin and Brame, 1983; Magdalinovic, 1989):

The material is packed to 700 cc volume using a vibrating table. This is the volumetric weight of the material to be used for grinding tests. For the first grinding cycle, the mill is started with an arbitrarily chosen number of mill revolutions. At the end of each grinding cycle, the entire product is discharged from the mill and is screened on a test sieve (Pi). Standard choice for P, is 106 micron. The oversize fraction is returned to the mill for the second run together with fresh feed to make up the original weight corresponding to 700 cc. The weight of product per unit of mill revolution, called the ore grindability of the cycle, is then calculated and is used to estimate the number of revolutions required for the second run to be equivalent to a circulating load of 250%. The process is continued until a constant value of the grindability is achieved, which is the equilibrium condition. This equilibrium condition may be reached in 6 to 12 grinding cycles. After reaching equilibrium, the grindabilities for the last three cycles are averaged. The average value is taken as the standard Bond grindability.

4 EXPERIMENTS

Firstly, Standard Bond's grindability tests were made for six limestone samples. Result of tests. Bond grindability values of limestone samples were appeared 6.14 g/rev, 2.89 g/rev, 2.58 g/rev, 2.48 g/rev, 2.42 g/rev and 1.54 g/rev, respectively. Then, the standard sets of grinding conditions used are shown in Table 2, for a laboratory mill of 6283 cm

452

volume. Eight mono-size fractions (-1.7+1.18, -1.18+0.850, - 0.850+0.600,-0.600+0.425, - 0.425 +0.300, - 0.300+ 0.212, - 0.212+0.150, -0.150+0.106 mm) were prepared and ground batch wise in a

laboratory-scale ball mill for determination of the specific rate of breakage. Each sample was taken out of the mill and dry sieved product size analysis.

Table 2. The standard set of grinding conditions.

Mill

Mill Speed

Balls

Matenal

Diameter Length Volume Critical Operational (0 = 75 90 Diameter (mm) Specific gravity Quality Assumed porosity Ball filling volume fraction (J ) Powder gravity, g/cm'

Interstitial filling (U%) Powder filling volume (f 9f )

G-1 2.78

G-2 2.76

200 mm 200 mm

6283 em-1

101 rprn 76 rpm

25.4 mm 78

Alloy Steel 40 %

20% (J = 0 2) G-3 2.65

Y-1 2.62

Y-2 2.63

52 5%(U = 0 525) 4.2 %( f =0.042)

Y-3 2.69

4.1 Determination of the specific rate of breakage

The first-order plots for various feed sizes of limestone samples are illustrated in Figure 1-6. The results indicated that grinding of all size fractions, six samples could be described by the first-order law. In additional, parameters of specific rate of breakage to supply by first-order plots are present in Table 3. The specific rates of breakage of each mono-size fraction that exhibited first-order grinding kinetic behaviour were determined from the slope of straight-line of first-order plots. Additional, Figure 7 shows the values of S, for grinding of the six different limestone samples, as a function of size.

4.2 Determination of B function

By definition, the values of B were determined from the size distributions at short grinding times. The parameters were determined according to the BII method (Austin et al, 1984), and show the graphical representation on Figure 8. Limestone samples show a typical normalised behaviour, and the progeny distribution does not depend on the particle size, and it followed that the parameter was zero. Model parameters supply by cumulative distribution and these parameters are presented in Table 3.

Table 3.Bond's gnndability values and characteristic breakage parameters tor samples of limestone.

Material

G-1 G-2 G-3 Y-1 Y-2 Y-3

Ghe gr/rev 6.14 2.89 2 58 2.48 2.42 1 54

S, (0.212-0.150 mm) (mm" )

1.15 0.69 0.67 0.63 0.53 0.50

ar (mm1) 4.01 2.61 2.79 2.11 2.30 0.87

a

0.785 0.988 1 161 1.564 1.178 0 228

Y

0.478 0.531 0.722 0 368 0.897 1.218

f.

0.51 0.38 0.30 0.24 0.32 0.41

1.199 1.509 1.716 1.699 1 571 1.712

453

454

5 VALIDATION OF THE RELATIONSHIPS BETWEEN BOND'S GRINDABILITY AND BREAKAGE PARAMETERS

5. / Variation of specific rate of breakagefS,) with Bond's grindability values(Gi,t)

For the same purposes, variation of specific rate of breakage (S,) with Bond's grindabilty (GhS) for six limestone samples was investigated, and it is shown in Figure 9. The values of S, seem to satisfy a linear with GbS with a correlation coefficient 0.96 that can be expressed as follows:

2 3 5

Bond GrindabllKy (gire

Figure 9. Variation of S, with GbS.

5J Varation of primary cumulative breakage constant () with Bond's grindability values (Gh)

For the same purposes, variation of primary cumulative breakage constant (/}) with Bond's grindabilty (Gi,t,) for six limestone samples was investigated, and it is shown in Figure II. The values of seem to satisfy a logarithmic with Ghf with a correlation coefficient 0.90 that can be expressed as follows:

Figure 11. Variation of with Gi,s.

5.2. Variation of first-order breakage constant (ar) with Bond's grindability values (Gi,K)

The values reported in Table 3 have been plotted in Fig, 10 referring to relation for different Gbs. The values of aj seem to satisfy a logarithmic with Gbf with a correlation coefficient 0.92 that can be expressed as follows:

5.4 Variation of primary cumulative breakage constant (y) with Bond's t>rindabilit\' values (GiJ

The values reported in Table 3 have been plotted in Fig. 10 referring to relation for different Gt,f. The values of y seem to satisfy a power with GbS with a correlation coefficient 0.78 that can be expressed as follows:

Figure 12. Variation of y with GhE.

455

6 CONCLUSIONS

The dry grinding of" size intervals of limestone samples showed that these samples followed the first-order breakage law with constant normalised primary breakage distribution function.

The values of the primary daughter fragment distributions and the values of a in S^orX" are different in the samples of limestone. As the amount of S, or ci]- values increase, the effective breakage increases, and breaks as very fast in the undersize of original particle size. The experimental values show that grinding is faster grinding for samples as fraction of bond grindability values (GhC) increase. Thus, Gl is faster grinding of original particle size than other samples of limestone.

The y value, which is the fineness factor, is lower for GI than other sample of limestone, indicating that more fines are produced in limestone grinding. Similarity, the Bond's grindability value (Ghg) for Gl, which is the easy grindability, is higher than other samples of l

Recommended